#------------------------------------------------------------------------------
#$Date: 2016-03-26 15:33:12 +0100 (Sat 26 de Mar de 2016) $
#$Revision: 180342 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/11/7201175.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7201175
loop_
_publ_author_name
'Kostakis, George E.'
'Chandra Mondal, Kartik'
'Abbas, Ghulam'
'Lan, Yanhua'
'Novitchi, Ghenadie'
'Buth, Gernot'
'Anson, Christopher E.'
'Powell, Annie K.'
_publ_section_title
;
 [Cu(N3)(p-CPA)]n: a two dimensional network exhibiting spin
 reorientation
;
_journal_issue                   10
_journal_name_full               CrystEngComm
_journal_page_first              2084
_journal_paper_doi               10.1039/b905707b
_journal_volume                  11
_journal_year                    2009
_chemical_formula_sum            'C9 H6 Cu N4 O3'
_chemical_formula_weight         281.72
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.368(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.4821(11)
_cell_length_b                   6.3061(6)
_cell_length_c                   14.7581(14)
_cell_measurement_reflns_used    3347
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      32.81
_cell_measurement_theta_min      3.99
_cell_volume                     1019.87(17)
_computing_cell_refinement       'Apex2 (Bruker AXS Inc., 2005)'
_computing_data_collection       'Apex2 (Bruker AXS Inc., 2005)'
_computing_data_reduction        'Apex2 (Bruker AXS Inc., 2003)'
_computing_molecular_graphics    'SHELXTL 6.14 (BrukerAXS Inc., 2003)'
_computing_publication_material  'SHELXTL 6.14 (BrukerAXS Inc., 2003)'
_computing_structure_refinement  'SHELXTL 6.14 (BrukerAXS Inc., 2003)'
_computing_structure_solution    'SHELXTL 6.14 (BrukerAXS Inc., 2003)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.962
_diffrn_measured_fraction_theta_max 0.866
_diffrn_measurement_device_type  'Bruker SMART Apex'
_diffrn_measurement_method       'CCD area detector'
_diffrn_radiation_monochromator  silicon
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.80000
_diffrn_reflns_av_R_equivalents  0.0208
_diffrn_reflns_av_sigmaI/netI    0.0314
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            4233
_diffrn_reflns_theta_full        28.75
_diffrn_reflns_theta_max         33.12
_diffrn_reflns_theta_min         3.99
_exptl_absorpt_coefficient_mu    2.967
_exptl_absorpt_correction_T_max  0.965
_exptl_absorpt_correction_T_min  0.854
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker AXS Inc., 2005)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.835
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             564
_exptl_crystal_size_max          0.09
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.01
_refine_diff_density_max         0.486
_refine_diff_density_min         -0.482
_refine_diff_density_rms         0.063
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     154
_refine_ls_number_reflns         2361
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.012
_refine_ls_R_factor_all          0.0263
_refine_ls_R_factor_gt           0.0244
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0416P)²+0.2787P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0681
_refine_ls_wR_factor_ref         0.0689
_reflns_number_gt                2181
_reflns_number_total             2361
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b905707b.txt
_cod_data_source_block           gek1
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               7201175
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.236046(19) 0.54388(3) 0.254333(12) 0.02150(9) Uani 1 1 d . . .
O1 O 0.31232(11) 0.46258(17) 0.38685(8) 0.0237(3) Uani 1 1 d . . .
O2 O 0.35504(11) 0.11464(17) 0.37652(7) 0.0248(2) Uani 1 1 d . . .
O3 O 0.41845(11) 0.46442(18) 0.57641(8) 0.0252(3) Uani 1 1 d . . .
C1 C 0.35750(14) 0.2879(2) 0.41979(10) 0.0209(3) Uani 1 1 d . . .
C2 C 0.42538(16) 0.2742(3) 0.52604(11) 0.0250(3) Uani 1 1 d . . .
H2A H 0.3908 0.1561 0.5540 0.030 Uiso 1 1 calc R . .
H2B H 0.5122 0.2411 0.5343 0.030 Uiso 1 1 calc R . .
C3 C 0.31406(16) 0.5071(3) 0.59771(11) 0.0243(3) Uani 1 1 d . . .
C4 C 0.31632(17) 0.6930(3) 0.65037(11) 0.0272(3) Uani 1 1 d . . .
H4A H 0.3871 0.7800 0.6670 0.033 Uiso 1 1 calc R . .
C5 C 0.21587(17) 0.7500(3) 0.67815(11) 0.0281(3) Uani 1 1 d . . .
H5A H 0.2170 0.8772 0.7129 0.034 Uiso 1 1 calc R . .
C6 C 0.11207(16) 0.6190(3) 0.65476(11) 0.0270(3) Uani 1 1 d . . .
C7 C 0.10972(17) 0.4350(3) 0.60110(12) 0.0288(4) Uani 1 1 d . . .
H7A H 0.0390 0.3479 0.5845 0.035 Uiso 1 1 calc R . .
C8 C 0.20915(16) 0.3792(3) 0.57206(11) 0.0275(3) Uani 1 1 d . . .
H8A H 0.2067 0.2552 0.5350 0.033 Uiso 1 1 calc R . .
C9 C 0.01135(17) 0.6664(3) 0.69166(12) 0.0291(4) Uani 1 1 d . . .
N1 N -0.06679(16) 0.6953(3) 0.72376(12) 0.0362(4) Uani 1 1 d . . .
N2 N 0.31816(14) 0.31431(19) 0.20505(9) 0.0233(3) Uani 1 1 d . . .
N3 N 0.33275(14) 0.3438(2) 0.12699(10) 0.0278(3) Uani 1 1 d . . .
N4 N 0.34966(18) 0.3769(3) 0.05597(11) 0.0389(4) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0043 0.0021 http://skuld.bmsc.washington.edu/scatter/AS_periodic.html
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0082 0.0043 http://skuld.bmsc.washington.edu/scatter/AS_periodic.html
O O 0.0142 0.0079 http://skuld.bmsc.washington.edu/scatter/AS_periodic.html
Cu Cu 0.2705 1.5628 http://skuld.bmsc.washington.edu/scatter/AS_periodic.html
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Cu1 O1 174.41(5) 2 . ?
O2 Cu1 N2 88.77(5) 2 2 ?
O1 Cu1 N2 90.60(5) . 2 ?
O2 Cu1 N2 88.68(5) 2 . ?
O1 Cu1 N2 93.17(5) . . ?
N2 Cu1 N2 166.68(4) 2 . ?
O2 Cu1 N1 93.26(5) 2 3_566 ?
O1 Cu1 N1 81.34(5) . 3_566 ?
N2 Cu1 N1 98.70(6) 2 3_566 ?
N2 Cu1 N1 94.50(6) . 3_566 ?
O2 Cu1 N1 85.99(5) 2 4_675 ?
O1 Cu1 N1 99.47(5) . 4_675 ?
N2 Cu1 N1 83.69(5) 2 4_675 ?
N2 Cu1 N1 83.10(5) . 4_675 ?
N1 Cu1 N1 177.49(5) 3_566 4_675 ?
C1 O1 Cu1 128.91(10) . . ?
C1 O2 Cu1 128.52(10) . 2_545 ?
C3 O3 C2 118.64(13) . . ?
O1 C1 O2 128.40(14) . . ?
O1 C1 C2 118.19(13) . . ?
O2 C1 C2 113.41(13) . . ?
O3 C2 C1 113.33(13) . . ?
O3 C2 H2A 108.9 . . ?
C1 C2 H2A 108.9 . . ?
O3 C2 H2B 108.9 . . ?
C1 C2 H2B 108.9 . . ?
H2A C2 H2B 107.7 . . ?
O3 C3 C4 115.06(15) . . ?
O3 C3 C8 124.82(15) . . ?
C4 C3 C8 120.12(17) . . ?
C5 C4 C3 120.19(16) . . ?
C5 C4 H4A 119.9 . . ?
C3 C4 H4A 119.9 . . ?
C4 C5 C6 119.71(16) . . ?
C4 C5 H5A 120.1 . . ?
C6 C5 H5A 120.1 . . ?
C7 C6 C5 119.83(17) . . ?
C7 C6 C9 120.05(17) . . ?
C5 C6 C9 119.98(16) . . ?
C8 C7 C6 120.61(16) . . ?
C8 C7 H7A 119.7 . . ?
C6 C7 H7A 119.7 . . ?
C7 C8 C3 119.50(16) . . ?
C7 C8 H8A 120.2 . . ?
C3 C8 H8A 120.2 . . ?
N1 C9 C6 176.57(19) . . ?
C9 N1 Cu1 132.57(14) . 3_566 ?
N3 N2 Cu1 124.15(11) . 2_545 ?
N3 N2 Cu1 116.57(10) . . ?
Cu1 N2 Cu1 107.03(7) 2_545 . ?
N4 N3 N2 177.38(19) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 O2 1.9535(11) 2 ?
Cu1 O1 1.9575(11) . ?
Cu1 N2 1.9692(13) 2 ?
Cu1 N2 1.9806(13) . ?
Cu1 N1 2.5557(17) 3_566 ?
Cu1 N1 2.9400(18) 4_675 ?
O1 C1 1.2525(18) . ?
O2 C1 1.2615(19) . ?
O2 Cu1 1.9535(11) 2_545 ?
O3 C3 1.354(2) . ?
O3 C2 1.4258(19) . ?
C1 C2 1.531(2) . ?
C2 H2A 0.9900 . ?
C2 H2B 0.9900 . ?
C3 C4 1.403(2) . ?
C3 C8 1.404(2) . ?
C4 C5 1.382(3) . ?
C4 H4A 0.9500 . ?
C5 C6 1.406(2) . ?
C5 H5A 0.9500 . ?
C6 C7 1.400(2) . ?
C6 C9 1.449(3) . ?
C7 C8 1.380(3) . ?
C7 H7A 0.9500 . ?
C8 H8A 0.9500 . ?
C9 N1 1.147(3) . ?
N1 Cu1 2.5557(17) 3_566 ?
N2 N3 1.2269(19) . ?
N2 Cu1 1.9692(13) 2_545 ?
N3 N4 1.141(2) . ?
